Differential scanning calorimetryThe technique was developed by E.S. Watsonand M.J. ONeill in 1960, and introducedcommercially at the Pittsburgh Conference onAnalytical Chemistry and AppliedSpectroscopy in 1963
Differential scanning calorimetry• This technique is used to study what happens to polymers/samples upon heating• It is used to study thermal transitions of a polymer/sample (the changes that take place on heating) – For example: • The melting of a crystalline polymer • The glass transition • The crystallization
Principle• The sample and reference are maintained at the same temperature, even during a thermal event in the sample• The energy required to maintain zero temperature difference between the sample and the reference is measured• During a thermal event in the sample, the system will transfer heat to or fro from the sample pan to maintain the same temperature in reference and sample pans
How studied what happens to a polymer when heated?The polymer is heated in a device that lookssomething like this:
• There are two pans, In sample pan, polymer is added, while the other, reference pan is left empty• Each pan sits on top of heaters which are controlled by a computer• The computer turns on heaters, and let them heat the two pans at a specific rate, usually 10oC/min.
• The computer makes absolutely sure that the heating rate stays exactly the same throughout the experiment
Why heaters don’t heat at the same rate?• The simple reason is that the two pans are different. One has polymer in it, and one doesnt. The polymer sample means there is extra material in the sample pan. Having extra material means that it will take more heat to keep the temperature of the sample pan increasing at the same rate as the reference pan
• So the heater underneath the sample pan has to work harder than the heater underneath the reference pan. It has to put out more heat. How much more heat it has to put out is what measured in DSC experiment?• Specifically, a plot is drawn as the temperature increases. The temperature is taken on x-axis whist the difference in heat output of the two heaters at a given temperature on y-axis
Differential Scanning Calorimetry Instrument• Two basic types of DSC instruments: power compensation DSC and heat-flux DSC Power compensation DSC Heat flux DSC
Power Compensation DSC individual heaters controller ∆Pintroduced in the early 1960s. sample reference pan pan Sample holder • Aluminum or Platinum pans inert gas inert gas vacuum vacuum Sensors thermocouple ∆T = 0 • Platinum resistance thermocouples • Separate sensors and heaters for the sample and reference Furnace • Separate blocks for sample and reference cells Temperature controller • Supply the differential thermal power to the heaters to maintain the temperature of the sample and reference at the program value
heating coilHeat Flux DSC Sample and reference holders sample pan reference pan• Al or Pt pans placed on constantan disc constantan• Sample and reference holders are chromel/alumel connected by a low-resistance wires heat flow path inert gas vacuum thermocouples ChromelSensors• Chromel® (an alloy made of 90% nickel and 10% chromium)-constantan area thermocouples (differential heat flow)• Chromel®-alumel (an alloy consisting of approximately 95% nickel, 2% manganese, 2% aluminium and 1% silicon) thermocouples (sample temperature) Thermocouple is a junction between two different metals that produces a voltage due to a temperature differenceFurnace• One block for both sample and reference cellsTemperature controller• The temperature difference between the sample and reference is converted to differential thermal power, which is supplied to the heaters to maintain the temperature of the sample and reference at the program value
DSC CalibrationBaseline• Evaluation of the thermal resistance of the sample and reference sensors• Measurements over the temperature range of interest 2-Step process • The temperature difference of two empty crucibles is measured • The thermal response is then acquired for a standard material, usually sapphire, on both the sample and reference platforms• Amplified DSC signal is automatically varied with the temperature to maintain a constant calorimetric sensitivity with temperature
Temperature• Goal is to match the melting onset temperatures indicated by the furnace Thermocouple readouts to the known melting points of standards analyzed by DSC• Should be calibrated as close as possible to the desired temperature rangeHeat flow• Use of calibration standards of known heat capacity, such as sapphire, slow accurate heating rates (0.5–2.0 °C/min), and similar sample and reference pan weights
Sample Preparation• Accurately-weigh samples (~3-20 mg)• Small sample pans (0.1 mL) of inert or treated metals (Al, Pt, Ni, etc.)• Several pan configurations, e.g., open, pinhole, or hermetically-sealed (airtight) pans• The same material and configuration should be used for the sample and the reference• Material should completely cover the bottom of the pan to ensure good thermal contact
• Avoid overfilling the pan to minimize thermal lag from the bulk of the material to the sensor * Small sample masses and low heating rates increase resolution Al Pt alumina Ni Cu quartz
DSC Curve• The result of a DSC experiment is a curve of heat flux versus temperature or versus time. There are two different conventions: exothermic reactions in the sample shown with a positive or negative peak, depending on the kind of technology used in the experiment.• This curve can be used to calculate enthalpies of transitions, which is done by integrating the peak corresponding to a given transition. The enthalpy of transition can be expressed using equation: ΔH = KA
• Where ΔH is the enthalpy of transition,• K is the calorimetric constant,• A is the area under the peak.• The calorimetric constant varies from instrument to instrument, and can be determined by analyzing a well-characterized material of known enthalpies of transition.• Area under the peak is directly proportional to heat absorbed or evolved by the reaction,• height of the peak is directly proportional to rate of the reaction
Factors affecting DSC curveTwo types of factors effect the DSC curve1-Instrumental factorsa- Furnace heating rateb- Recording or chart speedc- Furnace atmosphered- Geometry of sample holder/location of sensorse- Sensitivity of the recoding systemf-Composition of sample containers
2-Sample characteristicsa- Amount of sampleb- Nature of samplec- Sample packingd- Solubility of evolved gases in the samplee- Particle sizef- Heat of reactiong- Thermal conductivity
Determination of Heat Capacity• DSC plot can be used to determine Heat Capacity. Suppose a polymer is being heated. When we start heating two pans, the computer will plot the difference in heat output of the two heaters against temperature that is plot of heat absorbed by the polymer against temperature. The plot will look like this at first.
• The heat flow is heat (q) supplied per unit time (t), whereas,• The heating rate is temperature increase (ΔT) per unit time (t)
• By dividing heat flow (q/t) by the heating rate (ΔT/t). It ends up with heat supplied divided by the temperature increase, which is called heat capacity.
• When a certain amount of heat is transferred to the sample, its temperature increases by a certain amount, and the amount of heat it takes to get a certain temperature increase is called the heat capacity, or Cp, it can be figured up from the DSC plot
The Glass Transition Temperature• On further heating the polymer to a certain temperature, plot will shift downward suddenly, like this:
• This means there is more heat flow. There is an increase in the heat capacity of the polymer. This happens because the polymer has just gone through the glass transition. Because of this change in heat capacity that occurs at the glass transition, we can use DSC to measure a polymers glass transition temperature.• Take note that this change doesnt occur suddenly, but takes place over a temperature range. This makes picking one discreet Tg a kind of tricky matter, but we usually just take the middle of the incline to be the Tg.
Crystallization• After glass transition, the polymers have a lot of mobility. They wiggle and squirm, and never stay in one position for very long time. But when they reach the right temperature, they will give off enough energy to move into very ordered arrangements, which is called crystals.
• When polymers fall into these crystalline arrangements, they give off heat. When this heat is dumped out, it makes the little computer-controlled heater under the sample pan really happy. Its happy because it doesnt have to put out much heat to keep the temperature of the sample pan rising. You can see this drop in the heat flow as a big peak in the plot of heat flow versus temperature
The temperature at the highest point in the peak isusually considered to be the polymers crystallizationtemperature, or Tc
• Also, we can measure the area of the peak, which tells us the latent energy of crystallization of the polymer• But most importantly, this peak tells us that the polymer can in fact crystallize• If you analyze a 100% amorphous polymer, like polystrene, you wouldnt get this peak, because such materials dont crystallize• Also, because the polymer gives off heat when it crystallizes, we call crystallization is an exothermic transition
Melting• If we heat our polymer past its Tc, eventually well reach another thermal transition, called melting. When we reach the polymers melting temperature, Tm, the polymer crystals begin to fall apart, that is they melt. It comes out of their ordered arrangements, and begin to move around freely that can be spotted on a DSC plot
• Remember, the heat which polymer give off when crystallized is absorbed when reached at Tm. That is a latent heat of melting like latent heat of crystallization. When the polymer crystals melt, they must absorb heat in order to do so. Remember melting is a first order transition. This means that at the melting temperature, the polymers temperature wont rise until all the crystals have melted.
This means that the little heater under the sample panhas to put a lot of heat into the polymer in order to bothmelt the crystals and keep the temperature rising at thesame rate as that of the reference pan. This extra heatflow during melting shows up as a big dip on DSC plot,like this:
Putting It All Together• we saw a step in the plot when the polymer was heated past its glass transition temperature. Then we saw a big peak when the polymer reached its crystallization temperature. Then finally we saw a big dip when the polymer reached its melting temperature. To put them all together, a whole plot will often look something like this:
• Of course, not everything you see here will be on every DSC plot. The crystallization peak and the melting dip will only show up for polymers that can form crystals and melts.• Completely amorphous polymers wont show any crystallization, or any melting either. But polymers with both crystalline and amorphous domains, will show all the features
• From DSC plot you can see a big difference between the glass transition and the other two thermal transitions, crystallization and melting. For the glass transition, there is no dip, and theres no peak, either. This is because there is no latent heat given off, or absorbed, by the polymer during the glass transition. Both melting and crystallization involve giving off or absorbing heat.
• The only thing we do see at the glass transition temperature is a change in the heat capacity of the polymer.• Because there is a change in heat capacity, but there is no latent heat involved with the glass transition, we call the glass transition a second order transition. Transitions like melting and crystallization, which do have latent heats, are called first order transitions
How much crystallinity?• DSC can also tell us how much of a polymer is crystalline and how much is amorphous?• If we know the latent heat of melting, ΔHm, we can figure out the answer.• The first thing we have to do is to measure the peak area for the melting of a polymer. Since, DSC curve is a plot of heat flow per gram of material, versus temperature.• Heat flow (heat given off per second), so the area of the peak is given in units of heat x temperature x time-1 x mass-1 (joules x kelvins x (seconds)-1 x (grams)-1
• It can get simpler. We usually divide the area by the heating rate of dsc experiment. The heating rate is in units of K/s. So the expression becomes simpler:
• Now we have a number of joules per gram. But because we know the mass of the sample, we can make it further simpler. We just multiply this by the mass of the sample:Now we just calculate the total heat put on when the polymermelted. If we do the same calculation for peak on the DSC plot forthe crystallization of the polymer, we can get the total heatabsorbed by the heater during the crystallization. Well call theheat total heat of melting Hm, total, and total heat of thecrystallization Hc, total.Now were going to subtract the two:
• H is the heat absorbed by that part of the polymer which was already in the crystalline state before we heated the polymer above the Tc. We want to know how much of the polymer was crystalline before the experiment. Thats why we subtract the heat given off at crystallization.• From H we can figure up the percent crystallinity. It is divided by the specific heat of melting, Hm* which is the amount of heat absorbed by 1 g of a polymer. H is in joules, and the specific heat of melting is usually given in joules per gram, so the answer in grams, that is called mc
• This is the total amount of grams of polymer that were crystalline below the Tc. Now if we divide this number by the weight of our sample, mtotal, we get the fraction of the sample that was crystalline, and then of course, the percent crystallinity:
Liquid crystals• DSC is used in the study of liquid crystals. Some materials go from solid to liquid, they go through a third state, which displays properties of both the phases. This anisotropic liquid is known as a liquid crystalline state or mesomorphous state. Using DSC, it is possible to observe the small energy changes that occur as matter transitions from a solid to a liquid crystal and from a liquid crystal to anisotropic liquid.
Oxidative stability• To study the stability to oxidation of samples generally requires an airtight sample chamber. Usually, such tests are done isothermally (at constant temperature) by changing the atmosphere of the sample. First, the sample is brought to the desired test temperature under an inert atmosphere, usually nitrogen. Then, oxygen is added to the system. Any oxidation that occurs is observed as a deviation in the baseline. Such analysis can be used to determine the stability and optimum storage conditions for a material or compound.
Drug analysis• DSC is widely used in the pharmaceutical and polymer industries. For polymers, DSC is a handy tool for studying curing processes, which allows the fine tuning of polymer properties. The cross-linking of polymer molecules that occurs in the curing process is exothermic, resulting in a peak in DSC curve that usually appears soon after the glass transition.• In the pharmaceutical industry it is necessary to have well-characterized drug compounds in order to define processing parameters. For instance, if it is necessary to deliver a drug in the amorphous form, it is desirable to process the drug at temperatures below which crystallization can occur.
General chemical analysis• Melting-point depression can be used as a purity analysis tool when analysed by Differential scanning calorimetry. This is possible because the temperature range over which a mixture of compounds melts is dependent on their relative amounts. Consequently, less pure compounds will exhibit a broadened melting dip that begins at lower temperature than a pure compound.
Polymers• DSC is used widely for examining polymers to check their composition. Melting points and glass transition temperatures for most polymers are available from standard compilations, and the method can show up possible polymer degradation by the lowering of the expected melting point, which depends on the molecular weight of the polymer, so lower grades will have lower melting points than the expected.• Impurities in polymers can be determined by examining thermograms for anomalous peaks, and plasticizers can be detected at their characteristic boiling points.
Food science• In food science research, DSC is used in conjunction with other thermal analytical techniques to determine water dynamics. Changes in water distribution may be correlated with changes in texture.